TECHNETIUM METAL AND PYROMETALLURGICALLY FORMED SEDIMENTS
STUDY AND SPECIATION BY Tc-NMR AND EXAFS / XANES
Guerman K., Reich T., Sergeant C., Ortega R., Tarasov V., Simonoff M.
UMR 5084 / CNRS - Universite Bordeaux –1, Le Haut Vigneau, Gradignan, France
Eur.Synch.Rad.Facility, ROBL, Grenoble, France
Forschungszentrum Rossendorf, Institute for Radiochemistry, Dresden, Germany
Institute of Physical Chemistry and Institute of General and Inorganic Chemistry, R. A. S.
Abstract : EXAFS and NMR are being developed with respect to study and speciation of
technetium-99 in course of pyrometallurgical reprocessing of spent nuclear fuel. Based on the set of
standards including technetium metal, different techentium halogenides, oxohalogenides, oxydes and
pyrometallurgically formed sediments, Tc chemical forms responsible for Tc accumulation in fused
salts, deposits or gas-off depending on the applied reprocessing conditions are studying by means of
NMR and EXAFS. NMR spectrum of Tc metal powder obtained by FT of a free induction decay
accumulated after excitation of the spin system by a sequence of high frequency pulses (0.8 ìs) with a
dead time of 5.4 ìs and a repetition time of 1 ìs, provided with Knight shift K(ppm) = 7305 - 1.52 x
Tc) = 230 kHz at 293 K , CQ(99
Tc) = 5.52 MHz. EXAF spectra provided with excellent evidence
for Tc(IV) halogenides, but need further development for lower oxidation states of technetium.
Introduction : EXAFS and NMR are promising methods to enable us with speciation of
radioactive nuclides. It is important to use them for Tc speciation in pyrometallurgy which is now
considered as the most probable alternative approach to reprocessing of spent nuclear fuel.
Pyrometallurgy of uranium and plutonium in chloride and fluoride fused salts are now intensively
studied while little attention is given to long lived fission product technetium which is one of the
hazardous nuclear wastes. During pyrometallurgical spent fuel reprocessing, technetium can remain in
the fused salt or enter (depending on the applied temperatures, reagents and potentials) either the
sedimented phase contaminating Pu enriched phase, or electrodeposited U phase (Scheme 1). Neither
in sediment nor in deposit Tc phase could be detected by means of X-ray diffraction, Tc phase being
finely dispersed and X-ray amorphous. It is therefor very important to develop some other methods of
analyses like EXAFS and NMR applicable to Tc speciation in such samples.
Our preliminary results show that under such conditions Tc can also form several oxydes,
oxychlorides and chlorides of different but rather high volatility, turning on an important polluting risk
allied to gas-off .
The data on EXAF and NMR spectra of technetium being fragmentary and not presenting the
whole of the species possible in the pyrometallurgy conditions, it is of high importance to carry
synthetic work to supply a large set of technetium compounds in the closed containers which will meet
the security and quality demands, radioactivity level, special requirements on sample size, thickness,
Some EXAFS measurements of technetium solutions applicable in some content to
pyrometallurgcal treatment of spent nuclear fuel were presented earlier by [1, 2]. It provided with
EXAF data on technetium(IV) hexachloride in HCl solution. Recent studies however has given some
indication on the presence of unknown Tc chloride complex 
Tc metal and its binary alloys with vanadium have been studied earlier by 99
Tc NMR at
ambient temperature [4, 5, 6]. In these early works, the measurements were made in relatively low
magnetic fields (B0 1,4 T) in the differential passing mode with field sweep, which made difficult
the measurements of the anisotropic Knight shift (Kan). Moreover, the reported values of isotropic
Knight shift (K) for metal Tc varied from K= 6100 ppm in [4, 5] to K= 7150 ppm and Kan= 1160 ppm
Experimental : In this work EXAFS measurements are made at Radiochemical Hutch of
ROBL/ ESRF: beamsize of 3 x 20 mm2
, integrated flux at sample 6 x 1011 /s 200mA@ 20kEV,
spectral range 5 - 35 keV; 2/3 filling mode. Beam line control carried out with VME,SUN
workstation, SPEC Hot cells are used for sample positioning.
Tc NMR spectra of Tc metal powder at 120-400 K, technetium foil and some preliminary
results on the K(99
Tc) shifts in the alloy samples were recorded on a Bruker MSL-300
radiospectrometer in 7.04T magnetic field at 67.55 MHz resonance frequency.
Spectra NMR were obtained by FT of a free induction decay accumulated after excitation of
the spin system by a sequence of high frequency pulses (0.8 ìs) with a dead time of 5.4 ìs and a
repetition time of 1 ìs. The Knight shifts were measured relative to the external standard 0.1M KTcO4
Chemical preparations: All reagents were chemically pure grade. Technetium was
purchased as NH4TcO4 from Amersham Co. and as KTcO4 from V/O ISOTOP, RF and converted to
HTcO4 by cation exchange. N(CH3)4TcO4 was prepared as discribed in Tc metal was prepared by
reduction of tetramethylammonium pertechnetate N(CH3)4TcO4 (of 99.9% purity) in a flow of non-
explosive gas mixture 6% H2 in Ar in a quartz tube at 1150 K. Samples were cooled, crashed and the
80-150 ìm fraction was sieved of for NMR measurements. Same method was used for preparation of
the dispersed metal on metal oxide supports MgO, Al2O3, modified for evaporation of NH4TcO4 at the
later surface. To improve the resolution and accumulation NMR mode minimizing the electric
contacts, some technetium metal samples were dispersed in dodecane : apiezon (20 : 1) mixture and
Tc halogenides and oxydes were prepared as discribed in [8, 9]. Reference technetium
compounds prepared for EXAFS study : chlorides (M2TcCl6, M = Li, Na, K, R4N); fluorides,
(M2TcF6, M= H, Na, K); bromides ( M = Na, K, R4N); oxides TcO2, Tc4O5 and pertechnetates MTcO4
(M = Na, K, Cs, ); Samples of simulated pyrometallurgically reprocessed nuclear fuel (to be prepared):
Technetim hexachlorides in fused salts (chlorides and fluorides); Tc sublimated fraction; Tc
precipitated/deposit fraction (all with Tc-99 as the only radionuclide)
Results and discussion: The 99
Tc-NMR spectrum of polycrystalline metallic Tc comprises 8
symmetrically arranged satellites and the central component whose shape is governed by the Knight
shift anisotropy (Fig 2).
The distance in KHz between the first inner satellites is the lowest frequency of a quadruple
transition íQ. The line width of the central component at half-maximum was ~ 22 kHz at 293 K thus
having masked the effects of shift-anisotropy on the lineshape of the central transition (-1/2 +1/2).
At 400 K the line width is reduced and shows the axially – symmetric lineshape with K - K
= -809 ± 30 ppm.
Fig. 2 presents the temperature dependence of the isotropic Knight shift for technetium metal
powder, and Fig. 3 presents the temperature independence of the νQ for the same sample. This study
provided with K(ppm) = 7305 - 1.52 x
= 0.99. Experimental νQ(99
Tc) is 230 kHz at 293 K which
Tc) = 5.52 MHz. The latter is related to electric field gradient EFG (qexp
) by the equation:
] = 2.873*1022
, where Q = 0.3 barn.
In general, the total EFG at a nuclear site in a noncubic metal results from the addition of two
EFG parts, one being due to the lattice of the ionic core (enhanced by the Sternheimer antishielding
effect) and the other being due to the non-s-character of the conducting electrons:
In case of Tc, the contribution arising from the ionic core lattice may be interpolated from de
Wette’s  results for á = c/a = 1.604. We find that (1-ã)qlat
(at ã = -5 ). This
value is 52% of the experimental value obtained in the present work. This proportion is typical of the
most metals in which the (1-ã)qlat
contribution is ussually lower (in magnitude) than the observed one.
At the 99
Tc-NMR spectrum of Tc metal foil of 20 µm (Fig. 5), the central component is very
close to its position in Tc metal powder sample, but the 8 satellites are missed or not clear due to
highly defected crystal cell caused by mutual consecutive mechanic treatments. NMR and EXAFS
studies of dispersed Tc (supported on oxide matrix of MgO and Al2O3) and of Tc-Ru and Tc-Rh alloys
are in progress. NMR spectrum of the sample, sedimented from K2TcCl6 in NaCl-KCl melt at 550o
under reducing conditions formed by Ar-1%H2 bubbling, gave evidence for some metal state (9884
ppm) but also some to 30% of Tc(VII) (31 ppm).
Three main aspects under consideration with respect to EXAFS/XANES studies are the
following: 1) the ligand influence on the technetium EXAF spectra within the same Tc oxidation state
(F, Cl, Br, I and OH, H2O being the ligands of interest with respect to pyrometallurgy as a
reprocessing method), 2) the oxidation state including the lower and mixed oxidation states as well as
Tc cluster formation on the technetium EXAF spectra 3) cations on the technetium EXAF spectrum
within the same Tc oxidation state (Li, Na, K, Rb, Cs, Me4N, Et4N, Pr4N, Bu4N could be the cations of
interest , while TcO4
would be the anions under study (some preliminary results are
given in Fig. 6 and 7).
Tc K-edge k3
-weighted EXAFS and corresponding Fourier transform of the sample of
standard Tc(IV) halogenide (Me4N)2TcBr6 is present at Fig. 6. It resulted in the following EXAFS
Tc-Br N=5.8(2) ; R=2.51(2) Å ; σ2
= 0.0040 Å2
; ∆E0 = -16.9(5) eV
Six halogenide atoms and the distance found correspond well to the same parameters known
for similar compounds based on X-ray monocrystal analyses.
Tc K-edge k3
-weighted EXAFS and corresponding Fourier transform of the standard Tc(2,5+)
halogenide sample K3Tc2Cl8 is present in Fig. 7. The first coordination sphere of Tc in this compond
includes one Tc atom and four Cl atoms. EXAFS structural parameters for K3Tc2Cl8 (in such
preliminary approximation) resulted in the following values:
Tc-Tc N=1.6(3) R=2.20(2) Å σ2
Tc-Cl N=2.2(4) R=2.46(2) Å σ2
The overestimation of Tc-Tc intervention is evidently due to neglection of the four chlorine
atoms bounded to the second technetium atom. This correction of the model will be made in the
The results show excellent agreement in case of octahedral Tc(IV) bromide while for Tc
cluster compound an important difference between the experimental and the fit suppose that some
more chloride atoms but not only the first coordination sphere chlorides are influencing the EXAF
PPoossssiibbllee TTcc ssppeecciieess
iinn PPYYRROOCCHHEEMMIICCAALL RREEPPRROOCCEESSSSIINNGG
ooff ssppeenntt nnuucclleeaarr ffuueell
CONDITIONS IN FLOURIDE
IN FUSED SALT:
Tc METAL :
REDUCED Tc FLUORIDES
CONDITIONS IN CHLORIDE
IN FUSED SALT:
Tc METAL :
REDUCED Tc CHLORIDES
Fig 1. Radiochemical hutch of ROBL/ESRF
01 5 0 0 0 1 0 0 0 0 5 0 0 0 p p m
Fig 2. NMR-99
Tc spectrum of Tc metal powder ( Ô 80-150 ìm)
100 200 300 400 T, K
100 200 300 400
Fig.3. Temperature dependence of isotropic
Knight shift (K) for Tc metal powder
Fig.4. Temperature dependence of νQ for
Tc metal powder
Tc-NMR spectrum of Tc foil (d = 20 µm):
R + ∆ (Å)
Fig. 6. Tc K-edge k3
-weighted EXAFS and corresponding Fourier transform
of sample (Me4N)2TcBr6 : EXAFS structural parameters:
Tc-Br N=5.8(2) R=2.51(2) Å σ2
R + ∆ (Å)
Fig. 7. Tc K-edge k3
-weighted EXAFS and corresponding Fourier transform of sample
K3Tc2Cl8 EXAFS structural parameters for K3Tc2Cl8 (preliminary approximation):
Tc-Tc N=1.6(3) R=2.20(2) Å σ2
Tc-Cl N=2.2(4) R=2.46(2) Å σ2
1. K. Ben Said, M. Fattahi, Cl. Musikas, R.Revel , Speciation de Tc(IV) dans les solutions chlorees determinee
par spectroscopie d’absorption X (EXAFS). Comptes-rendus de Journees PRACTICE 1998, Villeneuve-les-
Avignon, 25-26 Fev. 1999.
2 . Revel R., Den Auwer C. Spectroscopie d’absorption X. Comptes-rendus de Journees PRACTICE 1998,
Villeneuve-les-Avignon, 25-26 Fev. 1999.
3 . Vichot L., Fattahi MM., Musikas C., Grambov B. Etude des formes reduites du technetium en milieu sulfato-
chlore. Comptes-rendus de Journees PRACTICE 1999, Villeneuve-les-Avignon, 17-18 Fev. 2000.
4. Jones W.H., Melford F. Phys. Rev. (1962) v.125, N 4, p.1253.
5 . Van Ostenburg, D.O., LammD., Trapp H.D., MacLead D.E./ Phys.Rev.(1962) v.128, N 4, p.1550
6. Van Ostenburg, D.O., Trapp H., LammD./ Phys.Rev. (1962) v.126, N 3 p.938.
7 . Guerman K.E., Kuzina A.F., Grigoriev M.S., GulevB.G., Spitzyn V.I. Synthesis and crystall structure of
Me4NTcO4. Proc. Acad. Sci.Russ. 1986.V.287, N.3, P. 650-653.
8. Guerman K.E., Grigor'ev M.S., Kuzina A.F., Spitsyn V.I. The structure and various physicochemical
properties of tetraalkylammonium pertechnetates. Russ.Journ. Inorg. Chem. 1987, v.32, N 5, p.667 - 670
(Engl.transl.); in Russ: p.1089 - 1095
9. Gerasimov V.N., Kryutchkov S.V., Guerman K.E., Kulakov V.M.,Kuzina A.F. X-ray photoelectron study of
structure of technetium compounds. In: Technetium and rhenium in chemistry and nuclear medicine. V.3.
Ed. by Nicolini M., Bandoly G., Mazzi U. New York: Raven Press, 1990. P.231-252.
10. De Wette F.W. Phys. Rev. (1961) v.123, N 1, p.103.
11. Tarasov V.P., Petrushin S.A., Privalov V.I. et all. Koord. Khim. (1986) v.12, N 9, p.713 (Engl. transl.)